### DEFORMATIONAL CALCULATION METHOD

### OF BEARING CAPABILITY OF FIBER-CONCRETE STEEL BENDING ELEMENTS

### ODKSZTAŁCENIOWA METODA OBLICZANIA NOŚNOŚCI ZGINANYCH ELEMENTÓW FIBROBETONOWYCH

### Z WŁÓKNAMI STALOWYMI

A b s t r a c t

This article proposes to use parabolic-linear diagram of deformation of steel fiber concrete under the conditions of compression. General principles of calculation method of steel fiber concrete elements. with the use of deformation diagrams of steel fiber concrete, have been submitted. The aim of this study was to present a method for calculating the deformation and deformation capacity steel fiber concrete bending elements based on the results of experimental studies. Results of tensile testing of samples allowed to put forward an analytical description of the time dependence of the stress-strain of steel fiber concrete in tension and compression, and accurately calculate the load and deflection bending elements. The experimental significance of the bearing capacity of steel fiber concrete bending elements on the fiber from the sheet and theoretical implications calculated by the proposed method have shown quite a good convergence.

*Keywords: steel fiber concrete, diagram, design, deformations*
S t r e s z c z e n i e

W artykule przedstawiono podstawowe zasady i metody obliczania zginanych elementów stalefibrobeto- nowych za pomocą paraboliczno-prostokątnych wykresów odkształceń stalefibrobetonu. Celem niniejszej pracy było zaproponowanie odkształceniowej metody obliczania nośności i odkształcenia stalefibrobetono- wyh elementów zginanych opartej na wynikach badań doświadczalnych. Wyniki badania próbek na rozcią- ganie pozwoliły na zasugerowanie analitycznego opisu wykresów zależności „naprężenie−odkształcenie”

stalefibrobetonu przy rozciąganiu i ściskaniu oraz dokładniejsze obliczenie nośności i ugięcia elementów zginanych. Doświadczalne wartości nośności stalefibrobetonowyh elementów zginanych z włóknami stalo- wymi i wartościami teoretycznymi obliczonymi według proponowanej metody wykazały dobrą zbieżność.

*Słowa kluczowe: stalefibrobeton, wykres, obliczenie, odkształcenie*

* Prof. Ph.D. Eng. Roman Kinash, AGH University of Science and Technology, Department of Geomechanics, Civil Engineering and Geotechnice; Lviv Polytechnic, Department of Architectural Constructions.

** Ph.D. Eng. Vitalij Bilozir, Department of Civil Engineering and Architecture, Lviv National Agrarian University.

**1. Introduction**

Exertion of fiber reinforcement to reinforce concrete allows us to enhance its exploitation qualities. These can include: lifted comparing to regular concrete resistance to cracking, firmness to stretching and pressure, frost resistance, shockproof, toughness to destruction etc. However, in case of changing diametrical reinforcement of beams and nets, which are used to reinforce the slabs, it is possible to reduce the labor intensity of the production of constructions.

So the calculation method of the bearing capacity of steel fiber elements is crucial [1, 2]

and has been elaborated by the analogy of reinforcement cement constructions. Thus at the stage of utmost balance, rectangular distribution diagrams of the strain of steel fiber concrete have been accepted in compact and stretch zones. The research, which has been conducted recently, has shown that such an approach is not fully reasoned and can lead to the situation when the constructions which were calculated according to the norms [1, 2], won’t meet the reliability requirements. Therefore, the improvement of the calculation method for steel fiber concrete bending elements on the basis of using whole diagrams of deformation of steel fiber concrete and reinforcement is a problem, the solving of which is explained below.

**2. Analysis of latest research and publications**

In this work [3] it is proposed to use parabolic-linear diagram of deformation of steel fiber
concrete under the conditions of compression. By the equation of a parabola, the ascending
*branch is described up to the level of strains, which are equal to temporary resistance f** _{fcc}*, and
to linear equations σ

_{fc}*= f*

*, in the rest of the diagram. The diagram, under the conditions of distension in the form of a parabola, the ascending branch and hyperbola or bilinear function, is at the descending. Experimentally received results concerning the diagram in assignment [3] haven’t been provided.*

_{fcc}The specialists of the German committee on concrete, offer an idealized diagram under
the extension of steel fiber concrete which is accepted as three-cornered [4]. The ascending
branch of this diagram is continuing as a horizontal line to deformations which equal
ε* _{fct}* = 3.5 · 10

^{–3}, descending branch is finishing under the deformations ε

*= 25 · 10*

_{fctu}^{–3}.

The work [5] has used the diagrams under extension and pressing, in a way of non-linear functions without descending branches.

Therefore, there is a list of propositions regarding the description of idealized diagrams, the parameters of which have not yet enough experimental explanation. Deformation diagrams are recommended to be used only at the stage of destruction, thus its criteria is to reach utmost deformation in concrete or reinforcement [3–5]. The aforementioned works didn’t consider such criteria as being upper bound of bearing capacity at the diagram “bending moment – flection”, which means the loss of balance abilities at the stretched and compressed zones of a bending element.

The aim of this work is to elaborate the deformation method of calculation of steel fiber concrete bending elements on the fiber of the sheet. The objectives of the research are the following: analytically describe whole diagrams of deformation of steel fiber concrete which were received in the assignment [6], elaborate mathematical apparatus to

calculate bearing capacity of steel fiber concrete bending elements, compare the results of the calculations and experimentally received data trying out steel fiber concrete bending samples of beam slabs.

**3. The method of calculating the deformation capacity of bending elements**
The proposed parameters of idealized diagrams when they are stretched or compressed
(Ill. 1) are well matched with the results of experimental research received in work [6]

and they have a lot in common with the appropriate parameters of hard constructional concrete [7].

Ill. 1. Idealized diagrams of deformation of steel fiber concrete on the fiber of the sheet under stress and stretching

Here is compression stress:

(1)

where:

η ε

*c* ε *fcc*

*fccu*

=

,1,

* a** _{k}* − polynomial coefficients;

− under the extension of ascending branch:

(2)
σ_{fcc}_{fcc}* _{k c}*η

^{k}*k*

*f* *a*

=

### ∑

= 1 5σ_{fct}_{fct}* _{k t}*η

^{k}*k*

*f* *a*

=

### ∑

= 1 5where:

η ε

*t* = *fct*

⋅ ^{−}
2 5 10. ^{3};

– at the descending branch:

(3)
*In the formulas (1), (2) the coefficients a** _{k}* are the polynomial coefficients which were
calculated by the method accepted at work [7] and takes into consideration the experimental
data [6]:

− at pressing:

− at stretching for ascending branch:

σ* _{fcc}*=

*f*

*( .1 525 210− ε*

_{fct}*)*

_{fct}*a* *E*

*f*

*fc fcc*
*fcc*
1=1 1. ε ,1

*a*_{2}= − − −1 *a a a a*_{1} _{3} _{4}− _{5}, *a*_{3}= −*a*_{1} 2*a*_{4}−3*a*_{5}−2

*a*_{4}=

### {

_{}

*k*−2

*a*

_{1}

### (

3^{γ}−2 12

### )

^{+}

^{γ}

^{−}6 2

_{ −}

*a*

_{5}

### (

10^{γ}

^{3}

^{−}9

^{γ}

^{+}2

### ) }

^{/}

_{}2 6

### (

^{γ}

^{2}

^{−}6 1

^{γ}

^{+}

### )

_{}

*a*_{5}=

### {

_{}

*k*−2

*a*

_{1}

### (

2^{γ}−3

^{γ}

### )

^{+}12

^{γ}

^{−}6

_{ −}

### (

^{γ}1

### )

^{2 2}

^{γ}

^{−}

^{}

_{}

^{β}

^{+}

*a*

_{1}

^{γ γ γ}

### (

2^{−}

^{2}

^{−}1

### )

^{+}

^{γ}

^{2}

^{(}2

^{γ}

^{−}3

^{)}

_{}

### (

^{−}

^{+}

### ) }

− +

### ( ) ^{(}

^{−}

^{)}

^{−}

### (

^{−}

^{+}

### ) (

^{−}

^{+}

### )

6 6 1 2

2 10 9 2 1 3 2 6 6 1

2

2 3 2 3 2

γ γ

γ γ γ γ γ γ γ γ

/

## {

## }

where:

− at pressing:

− average value at the stretching for ascending branch:

− at pressing:

γ ε

= ε^{fccu}

*fcc*
,
,
1
1

γ ε

= ε = ⋅

⋅ _{−}^{−} =

*fctu*
*fct*
,
,

.

. .

1 1

3 3

2 5 10

5 5 10 0 455

β ε

=1 1ε _{1}

1

. _{,}

,
*fccu*
*fcc*

− at stretching for ascending branch:

− at pressing:

– at stretching:

The formulas (1)−(3) describe quite precisely the diagrams of pressing and stretching
of steel fiber concrete up to the level of relative deformations which are 3·10^{–3}...4·10^{–3} at
the stretching and pressing. Theoretically received meaning of appropriate tensions, only at
certain dots, exceed the experimental ones at 0,3...3,5%, but in most cases they are less, thus
the equation (1)−(3) at first approximation can be used to evaluate the bearing capacity of
bending elements.

β = ⋅

⋅ ^{−}_{−} =
5 5 10
2 5 10. ^{3}_{3} 2 2

. .

*k* ^{fccu}

*fcc* *fccu*

*fcc*

= ⋅

− −

−

2 7 6 1 0 05

1

1

1 1

1

. , . .

, ,

,

ε

ε ε

ε

2

*k =* ⋅ ⋅

⋅

− −

⋅

⋅ −

−

− −

−

2 7 5 5 10

2 5 10 6 1 0 05

5 5 10 2 5 10 1

3

3 3

3

. .

. . .

. .

2 = −0 195.

Ill. 2. Distribution diagram of deformation and compression cross cut of bending steel fiber concrete element

In Ill. 2 the distribution diagram of deformation and compression of bending element, which is reinforced by fiber, is shown. Bending element which can accept the element equals:

*M = M*_{c}* + M*_{t1}* + M** _{t2}* (4)

*where: M*_{c}*, M*_{t1}*, M** _{t2}* − moments which are accepted by pressed and stretched zones according
to the diagram relative to the neutral axis. The results of the experiments and calculations

have proved as will be shown below that in the stretching zone at the stage of utmost balance, the third part of the work of fiber concrete for stretching due to the diagram (Ill. 1) can not be realized.

The balance of inner stresses is provided under the implementation of the conditions:

*N*_{c}* = N*_{t1}* + N** _{t2}* (5)

At ε_{c(2)}* ≤ 0.002, N** _{t2}* = 0.

Using the similarity of the triangles of the distribution diagram of deformation (Ill. 2) and known correlations of material resistance, it is possible to write for the compressed zone:

(6)

where

*N* *dF* *f* *a* *bdx*

*f* *a*

*c* *fc* *fcc* *k* *c*

*fcc*
*k*
*k*

*x*

*fcc* *k* *c*

= =

=

=

### ∑

=### ∫

### ∫

^{σ}

_{ε}

^{ε}

ε

,

( ( 1 1 5 0

1 1

)) ( ) ,

) (

+

=

= +

=

### ∑

### ∫ ∑

_{ε}

^{ε}

^{c}^{ε}

*fcc*
*k*

*fcc* *k*

*k*
*k*

*x* *x* *c*

*h* *bdx f b* *a*

*k*

2

1 1

5 1

5 0

1

1

1 )) ( )

,

( )

( ) ( )

+

+

ε +

ε

ε

ε ε

*c*
*fcc*

*k*
*c*

*c* *c*

*k*

*h*

2 *h*

1

1

1 2

1

*x* *c* *h*

*c* *c*

1 1

1 2

= +

ε

ε ε

( )

( ) ( )

(7)

Similarly by integrating for the stretching zone we receive:

(8)

(9)

(10)

(11)

*M* *xdF*

*f* *a* *x*

*h* *xbdx*

*c* *fc*

*fcc* *k* *c* *c*

*k* *fcc*

*k*

= =

= +

=

### ∫

### ∑

=σ

ε ε

ε
( _{( )} _{( )})

,

1 2

1 1

5 *ff b* *a*

*k* *h*

*h*

*fcc* *k*

*k*

*c* *c*

*fcc*
*k*

*c*

*c* *c*

+

+

+

### ∑

=_{2}1

5 1 2

1

1 1

ε ε

ε

ε

ε ε

( ) ( )

,

( ) ( ) (22

2 0

1

)

+

### ∫

*x* *k*

*N* *f b* *a*

*k* *h*

*t* *fct* *k* *h*

*k*

*c* *c*

*k*
*c*

1 1

5 1 2

3

3

1 2 5 10

2 5 10

= +

+

⋅

⋅

= −

### ∑

^{ε}

^{( )}

^{ε}

^{( )}

_{ε}−

. (

.

11 2

1 )+ ( )

+

ε_{c}

*k*

*M* *f b* *a*

*k* *h*

*t* *fct* *k* *h*

*k*

*c* *c*

*k*
*c*

1 1

5 1 2

3

3

2 2 5 10

2 5 10

= +

+

⋅

⋅

= −

### ∑

^{ε}

^{( )}

^{ε}

^{( )}

_{ε}−

. (

.

11 2

2 )+ ( )

+

ε_{c}

*k*

*N* *f bh* *h*

*t* *fct* *c*

*c* *c*

2 2 *c*

1 2

22

1 525 0 0025

105 0 0025

= −

+ − −

. ( _{( )} . ) .

( ) ( )

ε ( )

ε ε

ε ^{22}

1 2

ε_{c}_{( )}+ε_{c}_{( )}

*M* *f bh*

*t*

*fct* *c* *C*

*C*
2

2 22 2

3 2 3

0 7625 0 0025 70 0 0025

=

### (

^{.}

^{(}−

^{.}

^{)}−

^{(}−

^{.}

^{)}

### )

(

( ) ( )

(

ε ε

ε _{11}_{)}+ ε_{C}_{( )}_{2})^{2}

To reach ε_{c(2)}* = 0.0025, exertions N** _{t2}* = 0. The exertions at the stretched zone at this level:

(12)

(13)

**4. Comparative analysis of test results**

This analytical apparatus has been used to assess bearing capacity of steel fiber concrete
*elements of slab type within the sizes l = 700 mm, b = 200 mm, h = 30 mm. The samples *
have been tested at operating execution 600 mm with the application of concentrated
strengths at its thirds. The variations of percentage of fiber reinforcement of the volume
ρ_{fv}* and firmness of concrete-matrix f** _{c}* have been anticipated in the testing program. The
results of the testing (table 1) have proved that the norms [1] in which the rectangular
distribution diagrams of tension in compressed and stretched zones were accepted, don’t
allow to estimate precisely the bearing capacity of bending steel fiber concrete elements.

*Destructive bending moments M*_{exp}* have appeared to be essentially less than calculated M*_{[1]}

by the Norms [1]:

(14)

*Bending moments M** _{theor}* calculated under the proposed deformational method at
1...12% less than experimental ones. It is necessary to make a remark that the proposed
deformational method allows to receive data about the pressed deformational state of the
element during its work from the beginning of loading and up to its destruction. This way.

for example. for the samples of first series SFB−1.1 (samples SFB−1.1.1. SFB−1.1.2 and
SFB−1.1.3) have been received the following results which are given in the table 2 and in
the Ill. 3. For the samples of these series as it is seen in the table 2. the maximum bending
*moment M** _{theor}* = 110.31 Nm. ε

*= 0.000657. ε*

_{c(1)}*= 0.003. Thus. as we see. at the utmost stage of destruction. deformations appear in the almost resilient pressed fibers. At the level of stretched fibers. the deformations agree with the descending branch of the diagram. The criterion of the destruction of a particular sample is the loss of balance of inner efforts (maximum at the diagram ‘bending moment – flexures’).*

_{c(2)}*N* *dF* *f* *a* *bdx*

*f* *a*

*t* *fc* *fct* *k* *c*

*k*
*k*

*x*

*fct* *k* *c*

1 1

5 0

1

0 0025

= = 1

=

=

### ∑

=### ∫

### ∫

^{σ}

^{ε}

ε

.
( _{( )}++

⋅

=

+

+

=

=

### ∑

### ∫ ∑

^{ε}

^{c}^{ε}

*k*

*fct* *k*

*k*
*k*

*x* *x* *c*

*h* *bdx f b* *a*

*k*

( )) ( )

.

2

1 5 1

5 0

1

0 0025 1

1 εε ε

ε ε

*c*
*k*

*c*

*c* *c*

*k*

*h*

( ) ( )*h*

( ) ( )

.

2 1

1 2

1

0 0025

⋅

+

+

*M* *xdF*

*f* *a* *x*

*h* *xbdx*

*t* *fct*

*fct* *k* *c* *c*

*k*

*k*
1

1 2

1 5

0 0025

= =

= +

⋅

### ∫

### ∑

=σ

ε ε

( )

.

( ) ( ) ==

+

+

⋅

+

### ∑

=*f b* *a*

*k* *h*

*h*

*fct* *k*

*k*

*c* *c*

*k*
*c*

*c* *c*

2 0 0025

1

5 1 2 1

1

ε ε ε

ε ε

( ) ( ) ( )

( ) (

. 22

2 0

1

)

+

### ∫

*x* *k*

*M* *f* *f*

*f* *f*

*bh*

*fcc* *fct*

*fcc* *fct*

1

2

[ ]= ⋅ 2

+ ×

T a b l e 1
**Bearing capability of normal cuts of elements of slab type**

Sample name ρ_{fv}

[%] *f*_{fcc}

[MPa] *f*_{fct}

[MPa] *M*_{exp}

[Nm] *M*_{[1]}

[Nm] *M*_{theor}

[Nm]

SFВ−1.1.1

0.7 25.4 2.05

112.17

170.72 110.31

0.98

SFB−1.1.2 110.5 0.99

SFB−1.1.3 113.5 0.97

SFB−1.2.1

1.25 26.35 2.33

143.0

192.66 139.25

0.97

SFB−1.2.2 146.5 0.95

SFB−1.2.3 151.5 0.92

SFB−1.3.1

1.8 28.00 2.62

169.0

215.62 158.16

0.94

SFB−1.3.2 176.5 0.90

SFB−1.3.3 173.0 0.91

SFB−2.1.1

0.7 36.33 2.36

130.0

199.44 126.18

0.97

SFB−2.1.2 129.5 0.97

SFB−2.1.3 129.0 0.98

SFB−2.2.1

1.25 37.54 2.68

173.0

225.12 162.22

0.94

SFB−2.2.2 169.0 0.96

SFB−2.2.3 166.0 0.98

SFB−2.3.1

1.8 38.51 3.02

198.0

252.04 181.11

0.91

SFB−2.3.2 209.0 0.88

SFB−2.3.3 187.0 0.97

*M*
*M** ^{theor}*exp

Ill. 3.The correlation of theoretical meanings of incurvation from bending moment for the pattern of series SFB−1.1

T a b l e 2
**Calculation results of the pattern of series SFB−1.1**

ε* _{c(1)}* ε

*χ = (ε*

_{c(2)}*+ ε*

_{c(1)}

_{c(2)}*)/h*

*ΣX = 0*

*M*

*[Nm]*

_{theor}0 0 0 0 0

0.00009 0.00032645 0.0001388 4.33008E-05 22.9838465

0.0001 0.0003638 0.0001546 0.001746577 25.349335

0.0003 0.0011796 0.0004932 0.001398572 64.027182

0.0004 0.0016458 0.0006819 0.000767925 79.4477685

0.000584 0.0025 0.001028 0.000299537 104.988299

0.0006 0.0026 0.0010667 1.31868E-05 105.790229

0.000615 0.0027 0.0011051 0.000173637 107.967217

0.00063 0.0028 0.0011433 0.000410186 109.523891

0.000644 0.0029 0.0011813 0.000983105 110.00438

0.000657 0.003 0.0012192 7.21837E-05 110.312265

0.000671 0.0031 0.0012568 0.00035582 108.217099

0.000683 0.0032 0.0012943 0.000317555 103.160216

It is necessary to mention that calculations were being done with the use of the tabular processor Excel. Received data can also be used to calculate flexures. To accomplish this the use of Excel is needed and the dot chart “flexure – bending element” must be approximated by the equation of a straight line or parabola and then the flexures must be determined by Mohr’s integral.

**5. Conclusions**

1. Deformational calculation method of steel fiber concrete elements has been proposed and appropriate mathematical apparatus have been elaborated.

2. Experimental meaning of bearing capacity of steel fiber concrete bending elements on the fiber from the sheet and theoretical significance calculated by the proposed method have shown quite a good convergence (Table 1).

3. Bearing capacity of steel fiber concrete bending elements calculated by the method [1]

provided to the formula of which the experimental meanings of the firmness of steel fiber concrete at the extension and pressing is 28...54% higher than the experimentally received one. It is reasonable to make changes to the standard [1] to take the deformation method as the main method of calculation.

*This research work was performed as a part of the statutory investigations of AGH University of Science *
*and Technology in Cracow no. 11.100.197.*

R e f e r e n c e s

*[1] Конструкції будинків і споруд. Настанова з проектування та виготовлення *
*сталефібробетонних конструкцій: ДСТУ-Н Б В.2.6-78: 2009, Введ. в дію *
01.01.2010, К.: Мінрегіонбуд України, 2009, 43.

*[2] Сталефибробетонные конструкции: СП 52-104-2006, Введ. в действие 01.09.2006, *
М.: ФГУП “НИЦ «Строительство»”, 2007, 73.

*[3] Рак Н.А., Методика расчета сталефибробетонных конструкций с использованием *
*диаграмм деформирования сталефибробетона и стержневой арматуры, *
Материалы третьего Международного симпозиума “Проблемы современного бетона
и железобетона”, Минск, 09–11.11.2011, Режим доступу: http://www.belniis.by, 6.

*[4] Zilch K., Die DafStb- Richtlinie Stahlfaserbeton, Concrete Solutions 54. Betontage, *
K. Zilch,. J. Lingemann, 09–11 Februar 2011, Neu-Ulm, Режим доступу: http://www.

mb.bv.tum.de, 13.

*[5] Бабич Є.М., Робота і розрахунок згинальних сталефібробетонних елементів, *
Є.М. Бабич, С.Я. Дробишинець, Луцьк, Лнту 2012, 194.

*[6] Билозир В.В., Образование и раскрытие трещин в нормальных сечениях изгибаемых *
*сталефибробетонных элементов на фибре из листа, автореф. дис. на соиск. научн. *

степени к. т. н.: спец. 05.23.01/ В.В. Билозир, М.: НИИЖБ, 1991, 24.

*[7] Бамбура А.М., Експериментальні основи прикладної деформаційної теорії *
*залізобетону, автореф. дис. на здобуття наук. ступеня докт. техн. наук: спец. *

05.23.01/ А.М. Бамбура, Харків: ХДТУБА, 2006, 39.

*[8] Glinicki M.A., Beton ze zbrojeniem strukturalnym, XXV Ogólnopolskie Warsz-*
taty Pracy Projektanta Konstrukcji. Szczyrk, 10–13 marca, PZITB, Gliwice 2010,
279-308.